MANUFACTURE OF IRON. 39 



and precarious employment. This of course must have an effect ujiou the manufacturer ; and 

 it is not too much to say, tliat until this business is conducted with that science and skill which 

 are brought to bear upon it in other countries, there will be wanting in our case one important 

 element of success. 



A review of the processes of manufacture pur.siied in some parts of the Slate will, I think, 

 afford another clue to the causes which have served to depress this branch of industry ; and 

 as this is one of the most important topics connected with the practical part of this investiga- 

 tion, I trust that I shall be excused for entering somewhat in detail. 



In the description of the ores of iron which I have already given, it will be observed that 

 some of them are nearly pure ; that is, consist almost entirely of iron and oxygen in variable 

 proportions. Such are many of the ores found m the northern counties, in Orange county, 

 &c. As it is only necessary, in order to convert these pure minerals into metallic iron, that 

 they should be deprived of the oxygen which they contain, the reduction may be effected in a 

 very simple mamier. They are accordingly often mixed with a proper proportion of charcoal, 

 and subjected to heat in a low or Catalan forge. A part of the carbon, combining with the 

 oxygen of the ore, passes off in the form of carbonic acid gas ; while a variable proportion of 

 the carbon also combines with the iron, and causes the formation of cast iron, steel, or mal- 

 leable iron, according to circumstances. If the application of the heat be discontinued after 

 the fii-st reduction of the ore, the result will be cast iron ; but as the object in this case is 

 usually to obtain malleable iron by a single process, charcoal is added, and the heat continued 

 until the cast iron loses its liquidity, and is converted into a loup, as it is termed ; after which 

 it is brought under heavy hanuners, and formed into bars of various sizes and forms. When 

 a peculiar ore, as the spathic iron, is employed, the product of this process is an inferior 

 kind of steel. 



This forge is the most humble, and probably the oklest workshop of iron, and was formerly 

 in general use where the ores were sufficiently pure to admit of its employment. As it could 

 be erected at a trifling expense, it enabled the small capitalist to prosecute the manufacture 

 in situations where fuel was abundant, and it often employed the farmer in the intervals of 

 agricultural labor. These are perhaps the principal reasons why the forge is so generally 

 used in the northern part of the State. But I think it may be safely affirmed that its employ- 

 ment is wasteful ; and as fuel becomes less abundant, and capital increases, it must give place 

 to the improved furnace.* 



It is evident from the description of the process which has just been given, that the conver- 

 sion of the cast iron into malleable iron in tlie open forge, takes place during t'le free exposure 

 of the former to heat and air in contact with the combustible. There must, however, be great 

 waste both of fuel and of ore. Facts prove the correctness of this assertion. If I have been 

 correctly informed, three tons of the best ore, such as that from the Arnold mine, are required 

 for producing one ton of malleable iron ; and five hours is the average time consumed in carry- 



* See Col. Gibbs' Observations on liie Iron Works at Vergennes, Vennont. Urucc's Anierutm Mmtralogicat Journal, p. 80. 



